Infrared response of charge-coupled devicesMatthias Loch,a Ralf Widenhorn,a,† and Erik Bodegoma,b,‡abDepartment of Physics, Portland State University, Portland, OR 97207Department of Microelectronics, Delft University of Technology, 2628 CD Delft, NetherlandsABSTRACTWith a band gap of silicon of 1.1eV, the largest wavelength that can excite electrons from the valence to the conductionband is roughly 1100nm. As a consequence, in, for instance, a charge-coupled device, the quantum efficiency (QE) forwavelengths larger than 1100nm is assumed to be zero. We found that there is a response at those longer wavelengthsand that the response decreases with increasing wavelength. The QE increases with increasing chip temperature whichsuggests a thermally activated process. Impurities in the silicon provide the energy levels in the band gap, from whichelectrons can be excited either thermally or by absorption of a photon. It is these impurities that contribute to theinfrared response. We characterized the response at chip temperatures of 248 K to 293 K for wavelengths from 1200 nmto 1600 nm and calculated the activation energies at these wavelengths. We found that hot pixels, i.e., pixels withextraordinary high counts in a dark frame, tend to respond stronger to infrared light than normal pixels. This correlationgets stronger for longer wavelengths. It is argued that this response can be used for probing the impurities present in thesilicon bulk of the sensors.Keywords: CCD, infrared, impurities, activation energy1. INTRODUCTIONThe mode of action of a CCD imager is to convert photons hitting the imaging chip into electrons, which are stored andthen read out. The imaging chip is divided into individual elements, the pixels. The size and number of the pixelsdefines the spatial resolution of the camera. To characterize the light sensitivity of a CCD camera the QuantumEfficiency (QE) is used. It is the ratio of output and input and thus, describes the ability to convert incoming photonsinto measurable electrons. Generally, it is assumed that the QE for wavelengths longer than 1100 nm reduces to zero.1-4Hence, CCDs are not expected to respond in the near infrared range. At a first view this seems only logical. For siliconthe band gap between valence and conduction band is about 1.12 eV at room temperature. Hence, photons which carryless energy should not be able to excite electrons into the conduction band. Only light with wavelengths shorter thanapproximately 1100 nm, will be detected.In this paper, we will show experimental data with wavelengths from 1200 nm to 1600 nm. The results will show asmall but nevertheless measurable QE. The response is temperature dependent, suggesting a thermally activatedprocess. For such a process impurity or defect levels in the band gap might provide the intermediate states required forthe electrons to hop into the conduction band. Examples of such states are isolated vacancies, impurity atoms, anddislocations. A model will be presented to explain that process.A special relationship was found between hot pixels, i.e., pixels that have an intrinsically much higher dark current, andtheir infrared response. Hot pixels are distributed randomly over the CCD sensor. They are caused by defects orimpurities in the silicon chip. With increasing wavelength we found that hot pixels respond stronger to the infrared lightthan regular pixels.†‡Electronic mail: [email protected] mail: [email protected]
2. MEASUREMENTSIn this experiment a SBIG ST-8XE CCD (Santa Barbara Instrument Group) camera was studied. The sensor is KodakKAF-1602E, a 1530 by 1020 pixel array with individual pixel size of 9 x 9 microns and a full well capacity of 50,000electrons. A water cooled thermoelectric element is used to set and stabilize the temperature to an accuracy of 0.1 Kdown to approximately 50 K below ambient. The average dark current at 273 K was given by approximately1 electron/pixel/second.Monochromatic light in this experiment was obtained by the use of a monochromator made by Optometrics, modelMLM-2. It consists of a light source, a tungsten light bulb, a power supply, an iris and shutter, and an Optometrics MiniChrom monochromator. The monochromator is an in-line Fastie-Ebert monochromator. The light passes the iris, theslit, the monochromator and finally gets focussed by a lens onto the exit slit. On the way to the sensor three high passfilters cut out wavelengths smaller than 1200 nm. Two of them are located at the entrance and exit slits of themonochromator. The third filter is attached directly in front of the aperture of the camera and minimizes stray light. Forlonger wavelengths ( t 1350 nm) a band pass filter was placed between monochromator and the focussing lens. Thosefilters became necessary since the QE decreased significantly for longer wavelengths so that even photons atwavelengths of between 1200 nm and 1300 nm can significantly distort the results for the longer wavelengths. Inparticular, with the ruled gratings of the monochromator so-called Rowland ghosts typically appear due to periodicerrors in the spacing of the ruled grooves.5 The five band pass filters have center wavelengths of 1350, 1400, 1450,1500, and 1580 nm with a FWHM of approximately 25nm (Lambda Research Optics).To measure the QE of the system, absolute measurements of the incident irradiance are needed. A Germanium DetectorModule (GDM-1) from Optometrics is used; it consists of a mounted germanium photocell, integral low-noise highspeed operational amplifier, aperture assembly and housing. It has a photosensitive area of 5 mm in diameter. Thespectral range goes from 800 nm to 1800 nm.The results of the monochromator were compared with data obtained with a 1310 nm laser diode (a continuous light10 mW AlGaAs laser diode with a stable, single transverse mode oscillation). Another laser diode used was an InGaAsPsingle transverse mode Fabry-Perot laser with an optical output power of 6 mW and a peak emitting wavelength of 1520nm to 1580 nm. The same cut-off filters as in the previous experiment were used in the setup with diode lasers as the IRsource. For the InGaAsP laser an additional 1580nm band pass filter was used, because it seemed some light off thecentral wavelength was generated by the diode.For a given wavelength, ten temperatures were used from 248 K in increments of 5 K to 293 K. For each temperature awaiting period of thirty minutes for each 5 K step guaranteed that the temperature was stabilized. The exception was forthe InGaAsP laser, where in between 3 K steps, there was a two minute waiting time. All wavelengths within one dataset are exposed for the same time. Each series is measured with the same experimental setup with either themonochromator and the light bulb or the laser diode as light source.3. RESULTSFigure 1 shows the results for the QE at different temperatures for wavelengths from 1220 to 1290 nm. The data arecorrected for dark current and contain only the signal due to the IR radiation. One sees immediately the reason thatCCDs are not very useful in the NIR range above 1200 nm: the QE starts at 10-6 and drops to 10-7 at the higher end ofthis wavelength range. In the visible range the QE is close to one, or a difference between visible and infrared of sevenorders of magnitude. These results explain why the experiment has to be done with special care. For every photon ofvisible light it is at least 106 times easier to excite electrons into the conduction band. It is not possible to distinguishcounts between visible and infrared light and one has to be sure that the incoming light is really infrared light. One cansee that the QE decreases approximately exponentially with increasing wavelength. Most importantly, although onewould not expect a response for wavelengths longer than 1100 nm, one observes a wavelength and temperaturedependent response. The uncertainty in the individual data is approximately 20%. This might seem large, but in effectis mostly due to which part of the sensor is probed. An example of this can be seen in the data in Fig. 1. Alternating
wavelengths were obtained on different days; due to a rearrangement of the setup, the part of the sensor illuminated waschanged (only about 8,000 out of 1.5M pixels are illuminated in this setup). Hence, the data is specific to the part of thesensor illuminated. This is a possible indication that the localized defects play a role in the response. The model is thusone in which defects with energy levels in the band gap provide the mechanism to enable photons with energy less thanthe band gap to cause a response. Probing the IR response thus becomes a potential novel way to study defects insilicon.-14ln (QE)-15-16248 K258 K268 K278 K288 K293 K-17-18-191220124012601280wavelength [nm]Figure 1. The natural logarithm of the quantum efficiency as a function of wavelength at various temperatures.A linear fit is drawn to guide the eye.Figure 2 shows explicitly the temperature dependence at various wavelengths. It can be seen that for longer wavelengthsthe QE decreases significantly. The data for a given wavelength is done on the same part of the sensor and one noticesthat the data looks quite acceptable in the sense of the absence of scatter. These data lend credence to the explanation forthe scatter in the data in Fig. 1, since the Fig. 2 data were obtained on one part of the sensor. It is important to realizethat it is relatively easy for photons of 1220 nm to falsify measurements at a wavelength of 1290 nm. To studywavelengths longer than 1300 nm, the setup has to be modified from monochromator, light bulb, and high pass filtersbecause the QE will be extremely low.1.2e-61230124012501260127012701290Quantum 70280290Temperature [K]Figure 2. The dependence of the quantum efficiency on temperature for seven different wavelengths.
Looking at the results of the QE versus temperature, it seems as if the QE increases exponentially with the temperature.Since the response to the infrared light is temperature dependent, we can consider the activation energy of this process.Looking at the Arrhenius plot for a given wavelength (Fig. 3), one sees that a reasonable fit to the data is obtained. Thestraight line fit through these points brings out that there is a slight curvature in the data. A possible explanation is thatmultiple processes with different activation energies play a role.-14.0ln (QE)-14.5-15.0-220.127.116.11.18.104.22.168.0-11000/T [K ]Figure 3. Arrhenius plot for 1230 nm: the natural logarithm of the quantum efficiency vs. temperature.The IR-response, y, is approximately given by the following equation: yy0 exp 'E / kT with kT being the productof Boltzmann’s constant and the absolute temperature. The slope of the line in Fig. 3 gives the activation energy as:'E 238 meV.The same procedure can be used for the other wavelengths. As one can see in Fig. 4, the slope and hence the activationenergy, seems to decrease with increasing wavelength. That means that with longer wavelengths, and therefore smallerphoton energy, the activation energy gets smaller, too. It is to be observed that this is surprising. If simple (near-bandedge) impurities are the root cause, one would expect the activation energy to be the same for all wavelengths.-14ln 22.214.171.124.0-11000/T [K ]Figure 4. Arrhenius plots of natural logarithm of the quantum efficiency for wavelengths from 1220 nm to 1290 nm.In order to compare data sets for the various wavelengths and therefore different exposure times, one has to be sure thatthe exposure time has no influence on the activation energy. We have taken data for 30, 60, and 300 seconds exposure
time; the count rate or infrared response, stayed the same and the activation energies, within the noise margins, showedno change.As noted before, for longer wavelengths besides the monochromator, light bulb, and high pass filers, the band pass filterswere used. The activation energies were calculated as well for the wavelengths defined by the band pass filters (seeFig. 5). For data taken at different times under similar conditions, the activation energies varied. One has to note thatthe signals are extremely weak and therefore the analysis of the data is sensitive to all sorts of interferences (e.g., smallchanges in the light emission properties of the light bulb, vibrations of the setup, etc.). Hence we used laser diodes.The use of diodes has two main advantages. First of all, a laser diode insures that much less light, away from a single,narrow range of wavelengths, will be present. Second, one can achieve a higher intensity at these longer wavelengths.In order then to compare with the data at shorter wavelengths, one has to be sure that changes in intensity do not changethe activation energy. Therefore the intensity of the laser at 1315 nm was varied by a factor of ten and the activationenergies at the different power levels were calculated. The activation energies at those different intensities were withinthe experimental errors at that wavelength (4%).Figure 5 shows a summary of the data obtained using the light bulb and the laser diodes. The measured activationenergies decrease from 230 meV to 190 meV beyond about 1450nm. The laser diode data at 1310nm and the lightbulb data are in agreement. The InGaAsP laser diode was used with the band pass filter at 1570 nm. The spread in theactivation energy (see Fig. 5) for different data sets was much larger than for those with the light bulb. A possiblereason for this is that with the light bulb, extraneous, shorter wavelengths passed by the monochromator led to incorrectmeasurements. In effect we measured the activation energy associated with those extraneous and shorter wavelengths.For the spread in activation energy obtained with the diode, no pattern is discernible. Many reasons can be identified.First of all, the QE is extremely low. Although for most normal circumstances the diode provides a constant output, itdoes not. It fluctuates both in the dominant wavelength and in direction, thus a spread might occur in the measuredactivation energy. Due to the variable speckle pattern generated by the setup, the intensity can differ significantly fromone pixel to another. These fluctuations provide varying intensities at a pixel and increase the uncertainties associatedwith the measurements. For shorter wavelengths the overall non-uniformity was not significant. Potentially, at 1570 nmother impurities in the chip could be affected and therefore the intensity variations might become important. Thefluctuations in intensity and wavelength, the non-uniform illumination, the smaller area of the illumination, the weakersignal, and the shorter stabilization time of the temperature (two minutes after each 3 K change) all contribute to thespread in activation energy and the increased uncertainties at longer wavelengths.As mentioned previously the data from the light bulb beyond 1310 nm is suspect, quite possibly due to the phenomenonof Rowland ghosts. One observes clearly the much larger uncertainties at the longer wavelengths. To explore thevariations at these wavelengths, a more detailed study was made of the response of individual pixels.activation energy [meV]2402202001801601200Light bulbLaser diodes12501300135014001450150015501600wavelength [nm]Figure 5. Activation energy as a function of wavelength (data obtained with laser diodes are marked with the open circles).
There is a distinct relationship between hot pixels and infrared light. This relationship is more pronounced for longerwavelengths. We present data for a wavelength of 1580 nm. Hot pixels can be seen in each dark-frame. Defects areresponsible for the increased signal in these pixels.Figure 6 shows the dark count for individual pixels on the x-axis and the IR response of the respective pixel underillumination on the y-axis. This data set was taken at a temperature of 252 K for an exposure of 4 hours. 1365 pixelswere included in the k countsFigure 6. Counts in individual pixels under illumination of 1580 nm versus the dark count of those pixels at 252 K.One can see that there are two distinct and one diffuse regions. The first distinct region has a dark current of about 150to 350 and the second distinct region has a dark current of about 3000. The diffuse region contains some fifteen pixelsand has no discernable pattern. All of the pixels in the second region are hot pixels; all in the first one are normal pixels.Furthermore, one can see that the response of hot pixels is larger than that of the normal pixels. Of the twelve pixelswith counts over 20,000, 11 pixels are hot pixels. No other pixel on the whole chip did have a response that high. Thatmeans that the highest response is found in the area of the illumination and additionally that these pixels, except for one,are hot pixels.We also measured the average quantum efficiency at 1570 nm (see Fig. 7). The QE is much smaller than in the 1200 nmregime; in fact, it is six orders of magnitude smaller. Combined with Fig. 6, one can infer that the QE for hot pixelsmust be larger than for normal dark count pixels. The QE of hot pixels is about ten times larger than the average QE.Assuming that defects in individual hot pixels are the cause of the IR response, one can calculate the product of the crosssection (ı) and the number (N) of active defects present in the pixel. Nı equals the number of electrons counted dividedby the incident flux. Thus, the product Nı is equal to the area of the pixel times QE, and is approximately 8 u 10-18cm2. This is significantly less than the cross section responsible for ghosting.6 This is also much smaller than the defectcross sections associated with deep optical defects in semiconductors (10-16 cm2).7The activation energies associated with deep level defects in silicon are in a similar range of activation energies found inthis study.8 The cross sections measured here, are, however, significantly smaller. It is well known that if light causesan electronic excitation of such deep level defects, the local configuration changes. These changes are often metastable.We propose a model where such photoinduced defects are defects that can respond “normally” to light in the sense thatthey have a reasonable cross section. The decay of these defects prior to being hit by a second photon precludes electrongeneration. Because the decay times are so short, the effective cross section appears much smaller than the computedone. This model precludes a proportional response to the incident irradiance and instead it should be proportional to thesquare of the irradiance. Preliminary data show that the response has a dependence on irradiance stronger than linear at1570 nm. This model seems to be at variance to what was described earlier: defects in the band gap that are the directcause of the IR response. The complete model to explain all data is as follows.
Below about 1330 nm, defects in the gap are the main source of the response. Assuming that near band edge defects arethe main source, then with an activation energy on the order of 0.2 eV and a silicon band gap of 1.13 eV (at 273 K), onlyphotons more than 0.93 eV ( 1330 nm) are able to provide a direct signal. Impurities that have activation energies inthe relevant range include: In, Sn, C, Cu, Ti, Au, Zn, and Ni. These are all likely impurities. The model for these shorterwavelengths means that there should be a linear relationship between intensity and response. We have measured thiswith the laser at 1310 nm and an approximate linear relationship is indeed found. Above 1330 nm, an explanationinvolving metastable photoinduced defects is invoked to explain the extremely small cross sections.Quantum 0/T [K-1]Figure 7. The average quantum efficiency as a function of the inverse temperature at 1570nm.4. CONCLUSIONSSilicon CCDs respond to infrared light. Electrons are excited to the conduction band, although the energy of theincoming light is smaller than the band gap. This signal is temperature dependent and hence, the quantum efficiency istemperature dependent. The QE depends exponentially on the inverse temperature and thus the QE can be characterizedby an activation energy.The activation energy was measured with an increasing uncertainty at the longer wavelengths. This uncertainty is quitepossibly dependent on defects present in individual pixels and the difficulty in completely controlling the illumination.Nevertheless, a general trend is observable. The activation energies are in the range of 200 meV and seem to decreasefor the longer wavelengths.The quantum efficiency also decreases with increasing wavelength. For the shortest measured wavelength (1220 nm)the QE is in the range of 10-7 and for the longest measured wavelength (1580 nm) it is in the range of 10-13. The QEdecreases by a factor of 10-6. Compared to visible light with a QE close to one, these QEs are insignificant but are notequal to zero as normally is assumed.Based on the measurements a cross section was calculated at 1570 nm. This cross section is much smaller thanexpected. It is known that photoinduced defects are frequently metastable at room temperatures. The existence of theextremely small cross section can be explained by the fact that first a defect needs to be photoinduced and a secondphoton is needed to emit the electron into the conduction band. This is the model for the longer wavelengths. Forwavelengths less than about 1330 nm, defects in the band gap are the main source of the response. Potentially, thismethod might be used to probe the type of impurities present.It is the long integration times possible in CCDs, which makes it possible to probe defects in semiconductors heretoforenot easily accessible.
ACKNOWLEDGEMENTSWork supported by Technologiestichting STW. We thank Herman Peek, Albert Theuwissen, and Morley Blouke forfruitful discussions.REFERENCES:12345678J.R. Janesick, Scientific Charge-Coupled Devices, 172, SPIE-The International Society for Optical Engineering,Bellingham, WA, 2001A.J.P. Theuwissen, Solid-State Imaging with Charge-Coupled Devices, 298, Kluwer Academic Publishers,Amsterdam, 1996I. Glass, Handbook of Infrared Astronomy, 142, Cambridge University Press, New York, 1999D. E. Groom, S. E. Holland, M. E. Levi, N. P. Palaio, S. Perlmutter, R. J. Stover, and M. Wei, “Quantum Efficiency ofa Back-illuminated CCD Imager: An Optical Approach,” SPIE 3649, 80-90 (1999).F.A. Jenkins and H.E. White, Fundamentals of Optics, 370, 4th edition, McGraw Hill, New York, 1981A. Rest, L. Mündermann, R. Widenhorn, E. Bodegom, and T.C. McGlinn, “Residual images in charge-coupled devicedetectors,” Rev. Scient. Instr. 73, 2028 (2002)D. Redfield, and R. H. Bube, Photoinduced defects in semiconductors, 3, Cambridge University Press, New York,1996G.D. Watkins, “The Lattice Vacancy in Silicon,” Deep Centers in Semiconductors, ed. S.T. Pantelides, 177-214,Gordon and Breach Science Publishers, Philadelphia, 1992
MLM-2. It consists of a light source, a tungsten light bulb, a power supply, an iris and shutter, and an Optometrics Mini-Chrom monochromator. The monochromator is an in-line Fastie-Ebert monochromator. The light passes the iris, the slit, the monochromator and finally gets focussed by a le